CHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS


 Lily Johns
 2 years ago
 Views:
Transcription
1 CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is The APF is just the total sphere volumeunit cell volume ratio. For HCP, there are the equivalent of six spheres per unit cell, and thus 4π R V S 6 8π R Now, the unit cell volume is just the product of the base area times the cell height, c. This base area is just three times the area of the parallelepiped ACDE shown below. The area of ACDE is just the length of CD times the height BC. But CD is just a or R, and BC R cos (0 ) R
2 Thus, the base area is just AREA ()(CD)(BC) ()( R) R 6R and since c.6a R(.6) V C (AREA)(c) 6 R c (.S) (6 R ) ()(.6)R (.6) R Thus, APF V S V C 8π R (.6) R 0.74
3 Density Computations.8 Calculate the radius of an iridium atom, given that Ir has an FCC crystal structure, a density of.4 g/cm, and an atomic weight of 9. g/mol. We are asked to determine the radius of an iridium atom, given that Ir has an FCC crystal structure. For FCC, n 4 atoms/unit cell, and V C 6R (Equation.4). Now, ρ na Ir V C N A na Ir (6R )N A And solving for R from the above expression yields R na / Ir 6ρN A (4 atoms/unit cell) ( 9. g/mol) / (6)(.4 g/cm )(6.0 0 atoms/mol)( ) cm 0.6 nm
4 . Using atomic weight, crystal structure, and atomic radius data tabulated inside the front cover, compute the theoretical densities of lead, chromium, copper, and cobalt, and then compare these values with the measured densities listed in this same table. The c/a ratio for cobalt is.6. Since Pb has an FCC crystal structure, n 4, and V C 6R (Equation.4). Also, R 0.75 nm ( cm) and A Pb 07. g/mol. Employment of Equation.5 yields ρ na Pb V C N A (4 atoms/unit cell)(07. g/mol) {[ (6)( cm) ( ) ]/(unit cell) }(6.0 0 atoms/mol).5 g/cm The value given in the table inside the front cover is.5 g/cm. Chromium has a BCC crystal structure for which n and V C a 4 R (Equation.); also A Cr 5.00g/mol and R 0.5 nm. Therefore, employment of Equation.5 leads to ρ ( atoms/unit cell)(5.00 g/mol) (4)( cm) /(unit cell) (6.0 0 atoms/mol) 7.8 g/cm The value given in the table is 7.9 g/cm. Copper also has an FCC crystal structure and therefore ρ (4 atoms/unit cell)(6.55 g/mol) (6.0 0 atoms/mol) [()( cm)( ) ] /(unit cell) 8.90 g/cm
5 The value given in the table is 8.90 g/cm. Cobalt has an HCP crystal structure, and from the solution to Problem.6 (Equation.S), V C 6R c and, since c.6a and a R, c (.6)(R); hence V C 6R (.6)(R) (9.48)( )R (9.48)( )( cm) cm /unit cell Also, there are 6 atoms/unit cell for HCP. Therefore the theoretical density is ρ na Co V C N A (6 atoms/unit cell)(58.9 g/mol) ( cm /unit cell)(6.0 0 atoms/mol) 8.9 g/cm The value given in the table is 8.9 g/cm.
6 .6 Iodine has an orthorhombic unit cell for which the a, b, and c lattice parameters are 0.479, 0.75, and nm, respectively. (a) If the atomic packing factor and atomic radius are and 0.77 nm, respectively, determine the number of atoms in each unit cell. (b) The atomic weight of iodine is 6.9 g/mol; compute its theoretical density. (a) For indium, and from the definition of the APF APF V S V C n 4 π R abc we may solve for the number of atoms per unit cell, n, as n (APF) abc 4 π R Incorporating values of the above parameters provided in the problem state leads to (0.547)( cm)( cm)( cm) 4 π ( cm) 8.0 atoms/unit cell (b) In order to compute the density, we just employ Equation.5 as ρ na I abc N A (8 atoms/unit cell)(6.9 g/mol) {[ ( cm)( cm)( cm) ]/unit cell}(6.0 0 atoms/mol) 4.96 g/cm
7 Crystal Systems.0 Below is a unit cell for a hypothetical metal. (a) To which crystal system does this unit cell belong? (b) What would this crystal structure be called? (c) Calculate the density of the material, given that its atomic weight is 4 g/mol. (a) The unit cell shown in the problem statement belongs to the tetragonal crystal system since a b 0.0 nm, c 0.40 nm, and α β γ 90. (b) The crystal structure would be called bodycentered tetragonal. (c) As with BCC, n atoms/unit cell. Also, for this unit cell V C ( cm) ( cm).60 0 cm /unit cell Thus, using Equation.5, the density is equal to ρ na V C N A ( atoms/unit cell) (4 g/mol) ( cm /unit cell)(6.0 0 atoms/mol).0 g/cm
8 . Determine the indices for the directions shown in the following cubic unit cell: Direction A is a [0 ]direction, which determination is summarized as follows. We first of all position the origin of the coordinate system at the tail of the direction vector; then in terms of this new coordinate system x y z Projections 0a b c Projections in terms of a, b, and c 0 Reduction to integers not necessary Enclosure [0 ] Direction B is a [0] direction, which determination is summarized as follows. We first of all position the origin of the coordinate system at the tail of the direction vector; then in terms of this new coordinate system x y z Projections a b 0c Projections in terms of a, b, and c 0 Reduction to integers 0 Enclosure [0] Direction C is a [] direction, which determination is summarized as follows. We first of all position the origin of the coordinate system at the tail of the direction vector; then in terms of this new coordinate system
9 x y z a b Projections c Projections in terms of a, b, and c Reduction to integers Enclosure [] Direction D is a [] direction, which determination is summarized as follows. We first of all position the origin of the coordinate system at the tail of the direction vector; then in terms of this new coordinate system x y z a b Projections c Projections in terms of a, b, and c Reduction to integers Enclosure []
10 .4 Determine the Miller indices for the planes shown in the following unit cell: For plane A since the plane passes through the origin of the coordinate system as shown, we will move the origin of the coordinate system one unit cell distance to the right along the y axis; thus, this is a (4) plane, as summarized below. x y z Intercepts a c b Intercepts in terms of a, b, and c Reciprocals of intercepts Reduction 4 Enclosure (4) For plane B we will leave the origin at the unit cell as shown; this is a () plane, as summarized below. x y z a b Intercepts c Intercepts in terms of a, b, and c Reciprocals of intercepts Reduction not necessary Enclosure ()
11 .46 Consider the reducedsphere unit cell shown in Problem.0, having an origin of the coordinate system positioned at the atom labeled with an O. For the following sets of planes, determine which are equivalent: (a) (00), (00), and, ( 00) (b) ( 0), (0), (0 ), and ( 0) (c) ( ), ( ), ( ), and ( ) (a) The unit cell in Problem.0 is bodycentered tetragonal. Of the three planes given in the problem statement the (00) and (00) are equivalent that is, have the same atomic packing. The atomic packing for these two planes as well as the (00) are shown in the figure below.
12 (b) Of the four planes cited in the problem statement, ( 0) and ( 0) are equivalent to one another have the same atomic packing. The atomic arrangement of these planes is shown in the left drawing below. Furthermore, the (0) and (0) are equivalent to each other (but not to the other pair of planes); their atomic arrangement is represented in the other drawing. Note: the 0.44 nm dimension in the leftmost drawing comes from the relationship (0.0 nm) + (0.0 nm) [ ] /. Likewise, the nm dimension found in the rightmost drawing comes from [(0.0 nm) + (0.40 nm) ] /. (c) All of the ( ), ( ), ( ), and ( ) planes are equivalent, that is, have the same atomic packing as illustrated in the following figure:
13 .47 Here are shown the atomic packing schemes for several different crystallographic directions for some hypothetical metal. For each direction the circles represent only those atoms contained within a unit cell, which circles are reduced from their actual size. (a) To what crystal system does the unit cell belong? (b) What would this crystal structure be called? Below is constructed a unit cell using the six crystallographic directions that were provided in the problem.
14 (a) This unit cell belongs to the tetragonal system since a b 0.40 nm, c 0.50 nm, and α β γ 90. (b) This crystal structure would be called facecentered tetragonal since the unit cell has tetragonal symmetry, and an atom is located at each of the corners, as well as at the centers of all six unit cell faces. In the figure above, atoms are only shown at the centers of three faces; however, atoms would also be situated at opposite faces.
15 R..55 (a) Derive planar density expressions for BCC (00) and (0) planes in terms of the atomic radius (b) Compute and compare planar density values for these same two planes for vanadium. (a) A BCC unit cell within which is drawn a (00) plane is shown below. For this (00) plane there is one atom at each of the four cube corners, each of which is shared with four adjacent unit cells. Thus, there is the equivalence of atom associated with this BCC (00) plane. The planar section represented in the above figure is a square, wherein the side lengths are equal to the unit cell edge length, 4 R (Equation.); and, thus, the area of this square is just plane is just 4R 6 R. Hence, the planar density for this (00) PD 00 number of atoms centered on (00) plane area of (00) plane atom 6 R 6 R A BCC unit cell within which is drawn a (0) plane is shown below.
16 For this (0) plane there is one atom at each of the four cube corners through which it passes, each of which is shared with four adjacent unit cells, while the center atom lies entirely within the unit cell. Thus, there is the equivalence of atoms associated with this BCC (0) plane. The planar section represented in the above figure is a rectangle, as noted in the figure below. From this figure, the area of the rectangle is the product of x and y. The length x is just the unit cell edge length, which for BCC (Equation.) is 4 R. Now, the diagonal length z is equal to 4R. For the triangle bounded by the lengths x, y, and z Or y z x y (4 R) 4R 4 R Thus, in terms of R, the area of this (0) plane is just
17 Area(0) xy 4 R 4 R 6 R And, finally, the planar density for this (0) plane is just PD 0 number of atoms centered on (0) plane area of (0) plane atoms 6 R 8 R (b) From the table inside the front cover, the atomic radius for vanadium is 0. nm. Therefore, the planar density for the (00) plane is PD 00 (V) 6 R 6 (0. nm) 0.76 nm m While for the (0) plane PD 0 (V) 8 R 8 (0. nm) 5. nm m
18 .66 Figure.5 shows the first four peaks of the xray diffraction pattern for copper, which has an FCC crystal structure; monochromatic xradiation having a wavelength of 0.54 nm was used. (a) Index (i.e., give h, k, and l indices) for each of these peaks. (b) Determine the interplanar spacing for each of the peaks. (c) For each peak, determine the atomic radius for Cu and compare these with the value presented in Table.. (a) Since Cu has an FCC crystal structure, only those peaks for which h, k, and l are all either odd or even will appear. Therefore, the first peak results by diffraction from () planes. (b) For each peak, in order to calculate the interplanar spacing we must employ Equation.. For the first peak which occurs at 4.8 d nλ sin θ ()(0.54 nm) () sin nm (c) Employment of Equations.4 and. is necessary for the computation of R for Cu as R a (d hkl) (h) + (k) + (l) (0.067 nm) () + () + () 0.66 nm
19 Similar computations are made for the other peaks which results are tabulated below: Peak Index θ d hkl (nm) R (nm)
MAE 20 Winter 2011 Assignment 2 solutions
MAE 0 Winter 0 Assignment solutions. List the point coordinates of the titanium, barium, and oxygen ions for a unit cell of the perovskite crystal structure (Figure.6). In Figure.6, the barium ions are
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationA crystalline solid is one which has a crystal structure in which atoms or ions are arranged in a pattern that repeats itself in three dimensions.
CHAPTER ATOMIC STRUCTURE AND BONDING. Define a crstalline solid. A crstalline solid is one which has a crstal structure in which atoms or ions are arranged in a pattern that repeats itself in three dimensions..2
More informationCrystal Symmetries METE 327 Physical Metallurgy Copyright 2008 Loren A. Jacobson 5/16/08
Crystal Symmetries Why should we be interested? Important physical properties depend on crystal structure Conductivity Magnetic properties Stiffness Strength These properties also often depend on crystal
More informationChapter 3: The Structure of Crystalline Solids
Sapphire: cryst. Al 2 O 3 Insulin : The Structure of Crystalline Solids Crystal: a solid composed of atoms, ions, or molecules arranged in a pattern that is repeated in three dimensions A material in which
More informationRelevant Reading for this Lecture... Pages 8387.
LECTURE #06 Chapter 3: Xray Diffraction and Crystal Structure Determination Learning Objectives To describe crystals in terms of the stacking of planes. How to use a dot product to solve for the angles
More informationCrystals are solids in which the atoms are regularly arranged with respect to one another.
Crystalline structures. Basic concepts Crystals are solids in which the atoms are regularly arranged with respect to one another. This regularity of arrangement can be described in terms of symmetry elements.
More informationChapter Outline. How do atoms arrange themselves to form solids?
Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Simple cubic Facecentered cubic Bodycentered cubic Hexagonal closepacked
More informationChapter 3: Structure of Metals and Ceramics. Chapter 3: Structure of Metals and Ceramics. Learning Objective
Chapter 3: Structure of Metals and Ceramics Chapter 3: Structure of Metals and Ceramics Goals Define basic terms and give examples of each: Lattice Basis Atoms (Decorations or Motifs) Crystal Structure
More informationChapters 2 and 6 in Waseda. Lesson 8 Lattice Planes and Directions. Suggested Reading
Analytical Methods for Materials Chapters 2 and 6 in Waseda Lesson 8 Lattice Planes and Directions Suggested Reading 192 Directions and Miller Indices Draw vector and define the tail as the origin. z Determine
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationExperiment: Crystal Structure Analysis in Engineering Materials
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of Xray diffraction techniques for investigating various types
More informationChapter 2 Crystal Lattices and Reciprocal Lattices
Chapter 2 Crystal Lattices and Reciprocal Lattices Abstract In this chapter, the basic unit vectors in real space and the basic unit vectors in reciprocal space, as well as their reciprocal relationships,
More informationChapter 3. 1. 3 types of materials amorphous, crystalline, and polycrystalline. 5. Same as #3 for the ceramic and diamond crystal structures.
Chapter Highlights: Notes: 1. types of materials amorphous, crystalline, and polycrystalline.. Understand the meaning of crystallinity, which refers to a regular lattice based on a repeating unit cell..
More informationCrystal Structure Determination I
Crystal Structure Determination I Dr. Falak Sher Pakistan Institute of Engineering and Applied Sciences National Workshop on Crystal Structure Determination using Powder XRD, organized by the Khwarzimic
More informationv kt = N A ρ Au exp (
42 4.2 Determination of the number of vacancies per cubic meter in gold at 900 C (1173 K) requires the utilization of Equations 4.1 and 4.2 as follows: N v N exp Q v N A ρ Au kt A Au exp Q v kt (6.023
More informationBasic Concepts of Crystallography
Basic Concepts of Crystallography Language of Crystallography: Real Space Combination of local (point) symmetry elements, which include angular rotation, centersymmetric inversion, and reflection in mirror
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide
More informationSolid State Theory Physics 545
Solid State Theory Physics 545 CRYSTAL STRUCTURES Describing periodic structures Terminology Basic Structures Symmetry Operations Ionic crystals often have a definite habit which gives rise to particular
More informationSolid State Device Fundamentals
Solid State Device Fundamentals ENS 345 Lecture Course by Alexander M. Zaitsev alexander.zaitsev@csi.cuny.edu Tel: 718 982 2812 Office 4N101b 1 Solids Three types of solids, classified according to atomic
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationThe University of Western Ontario Department of Physics and Astronomy P2800 Fall 2008
P2800 Fall 2008 Questions (Total  20 points): 1. Of the noble gases Ne, Ar, Kr and Xe, which should be the most chemically reactive and why? (0.5 point) Xenon should be most reactive since its outermost
More informationXray diffraction: theory and applications to materials science and engineering. Luca Lutterotti
Xray diffraction: theory and applications to materials science and engineering Luca Lutterotti luca.lutterotti@unitn.it Program Part 1, theory and methodologies: General principles of crystallography
More informationIt is possible to map the surfaces of conducting solids at the atomic level using an
3 C H A P T E R Crstal Structures and Crstal Geometr It is possible to map the surfaces of conducting solids at the atomic level using an instrument called the scanning tunneling microscope (STM). The
More informationReading. Chapter 12 in DeGraef and McHenry Chapter 3i in Engler and Randle
Class 17 Xray Diffraction Chapter 1 in DeGraef and McHenry Chapter 3i in Engler and Randle Reading Chapter 6 in DeGraef and McHenry (I WILL ASSUME THAT YOU KNOW ABOUT THIS CONCEPT ALREADY! IF NOT, READ
More informationEXPERIMENT 4. Microwave Experiments. Introduction. Experimental Procedure. Part 1 : Double Slit
EXPERIMENT 4 Microwave Experiments Introduction Microwaves are electromagnetic radiation in the centimeter range of wavelengths. As such, they, like light, will exhibit typical wave properties like interference
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationLecture 2. Surface Structure
Lecture 2 Surface Structure Quantitative Description of Surface Structure clean metal surfaces adsorbated covered and reconstructed surfaces electronic and geometrical structure References: 1) Zangwill,
More informationCrystallographic Directions, and Planes
Crstallographic Directions, and Planes Now that we know how atoms arrange themselves to form crstals, we need a wa to identif directions and planes of atoms. Wh? Deformation under loading (slip) occurs
More informationThe Crystal Structures of Solids
The Crystal Structures of Solids Crystals of pure substances can be analyzed using Xray diffraction methods to provide valuable information. The type and strength of intramolecular forces, density, molar
More informationHW1. N = ρv/m =
1 HW1 1. Two spheres are cut from a certain uniform rock. One has radius r=5.0 cm. The mass of the other is eight times greater. Find its radius R. Since mass radius 3 R = r 8 1/3 = 10cm 2. The mass of
More informationLAB #1 THE CRYSTALLOGRAPHY AND MILLER INDICES
LAB #1 THE CRYSTALLOGRAPHY AND MILLER INDICES THE OBJECTIVES: 1. To study simple crystal lattices using a simulation packages. THE THEORY: Solid state semiconductor technology has brought valuable systems
More informationXRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US. Hanno zur Loye
XRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US Hanno zur Loye Xrays are electromagnetic radiation of wavelength about 1 Å (1010 m), which is about the same size as an atom. The
More informationComposition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
More informationElementary Crystallography for XRay Diffraction
Introduction Crystallography originated as the science of the study of crystal forms. With the advent of the xray diffraction, the science has become primarily concerned with the study of atomic arrangements
More informationRetained Austenite: NonDestructive Analysis by XRD and ASTM E Dr. Alessandro Torboli  XRay Marketing Manager
Retained Austenite: NonDestructive Analysis by XRD and ASTM E97503 Dr. Alessandro Torboli  XRay Marketing Manager Outline Introduction to XRay Diffraction Retained Austenite Retained Austenite by
More informationCHEM 10113, Quiz 7 December 7, 2011
CHEM 10113, Quiz 7 December 7, 2011 Name (please print) All equations must be balanced and show phases for full credit. Significant figures count, show charges as appropriate, and please box your answers!
More informationSample Exercise 12.1 Calculating Packing Efficiency
Sample Exercise 12.1 Calculating Packing Efficiency It is not possible to pack spheres together without leaving some void spaces between the spheres. Packing efficiency is the fraction of space in a crystal
More informationa a. θ = cos 1 a b ) b For nonzero vectors a and b, then the component of b along a is given as comp
Textbook Assignment 4 Your Name: LAST NAME, FIRST NAME (YOUR STUDENT ID: XXXX) Your Instructors Name: Prof. FIRST NAME LAST NAME YOUR SECTION: MATH 0300 XX Due Date: NAME OF DAY, MONTH DAY, YEAR. SECTION
More informationCrystal Structure. A(r) = A(r + T), (1)
Crystal Structure In general, by solid we mean an equilibrium state with broken translation symmetry. That is a state for which there exist observables say, densities of particles with spatially dependent
More informationCHAPTER 3: CRYSTAL STRUCTURES
CHAPTER 3: CRYSTAL STRUCTURES Crystal Structure: Basic Definitions  lecture Calculation of material density selfprep. Crystal Systems lecture + selfprep. Introduction to Crystallography lecture + selfprep.
More informationIf a question asks you to find all or list all and you think there are none, write None.
If a question asks you to find all or list all and you think there are none, write None 1 Simplify 1/( 1 3 1 4 ) 2 The price of an item increases by 10% and then by another 10% What is the overall price
More informationChapter 15 Mensuration of Solid
3 Chapter 15 15.1 Solid: It is a body occupying a portion of threedimensional space and therefore bounded by a closed surface which may be curved (e.g., sphere), curved and planer (e.g., cylinder) or
More informationPOWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS
EXPERIMENT 4 POWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS I. Introduction The determination of the chemical structure of molecules is indispensable to chemists in their effort
More informationLECTURE SUMMARY September 30th 2009
LECTURE SUMMARY September 30 th 2009 Key Lecture Topics Crystal Structures in Relation to Slip Systems Resolved Shear Stress Using a Stereographic Projection to Determine the Active Slip System Slip Planes
More information1. By how much does 1 3 of 5 2 exceed 1 2 of 1 3? 2. What fraction of the area of a circle of radius 5 lies between radius 3 and radius 4? 3.
1 By how much does 1 3 of 5 exceed 1 of 1 3? What fraction of the area of a circle of radius 5 lies between radius 3 and radius 4? 3 A ticket fee was $10, but then it was reduced The number of customers
More informationPAPER CRYSTAL STURCTURE Put your name and period on structure near the name of the crystal. Cut along SOLID lines. Fold inward along DASH lines so
PAPER CRYSTAL STURCTURE Put your name and period on structure near the name of the crystal. Cut along SOLID lines. Fold inward along DASH lines so that your name and crystal s name is visible. Put your
More informationCrystallographic Points, Directions, and Planes. ISSUES TO ADDRESS... a v. Points, Directions, and Planes in Terms of Unit Cell Vectors
Crstallographic Points, Directions, and Planes. Points, Directions, and Planes in Terms of Unit Cell Vectors ISSUES TO ADDRESS... How to define points, directions, planes, as well as linear, planar, and
More informationEngr Materials Science and Engineering TEST 4  Sample Solution
Engr 70  Materials Science and Engineering TEST 4  Sample Solution Part : Solve each of the following problems completely. 1. In this problem we are asked to show that the minimum cationtoanion radius
More informationTheory of XRay Diffraction. Kingshuk Majumdar
Theory of XRay Diffraction Kingshuk Majumdar Contents Introduction to XRays Crystal Structures: Introduction to Lattices Different types of lattices Reciprocal Lattice Index Planes XRay Diffraction:
More informationBasics in Xray Diffraction and Special Application
Basics in Xray Diffraction and Special Application Introduction: Xray Diffraction (XRD) helps one to reach the science at atomic scale in the analysis of crystal structure, chemical composition, and
More informationCatholic Schools Trial Examination 2004 Mathematics
0 Catholic Trial HSC Examination Mathematics Page Catholic Schools Trial Examination 0 Mathematics a If x 5 = 5000, find x correct to significant figures. b Express 0. + 0.. in the form b a, where a and
More informationChem 106 Thursday Feb. 3, 2011
Chem 106 Thursday Feb. 3, 2011 Chapter 13: The Chemistry of Solids Phase Diagrams  (no BornHaber cycle) 2/3/2011 1 Approx surface area (Å 2 ) 253 258 Which C 5 H 12 alkane do you think has the highest
More informationVECTOR NAME OF THE CHAPTER PARTC FIVE MARKS QUESTIONS PARTE TWO OR FOUR QUESTIONS PARTA ONE MARKS QUESTIONS
NAME OF THE CHAPTER VECTOR PARTA ONE MARKS QUESTIONS PARTB TWO MARKS QUESTIONS PARTC FIVE MARKS QUESTIONS PARTD SIX OR FOUR MARKS QUESTIONS PARTE TWO OR FOUR QUESTIONS 1 1 1 1 1 16 TOTAL MARKS ALLOTED
More informationReview for Final  Geometry B
Review for Final  Geometry B Multiple Choice Identify the choice that best completes the statement or answers the question. 1. A model is made of a car. The car is 4 meters long and the model is 7 centimeters
More informationImperfections in atomic arrangements
MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification
More informationNext, solid silicon is separated from other solid impurities by treatment with hydrogen chloride at 350 C to form gaseous trichlorosilane (SiCl 3 H):
University Chemistry Quiz 5 2014/12/25 1. (5%) What is the coordination number of each sphere in (a) a simple cubic cell, (b) a bodycentered cubic cell, and (c) a facecentered cubic cell? Assume the
More informationFigure 1. Torsion angle φ = Tor (p 1, p 2, p 3, p 4 ). The angle is measured in the plane perpendicular to b = p 3 p 2.
6. Torsion angles and pdb files In the study of space curves, the Frenet frame is used to define torsion and curvature, and these are used to describe the shape of the curve. A long molecule such as DNA
More informationESS 212: Laboratory 2 and 3. For each of your paper models, assign crystallographic axes that will serve to orient the model.
ESS 212: Laboratory 2 and 3 Lab Topics: Point groups of symmetry Crystal systems and Crystallographic axes Miller Indices of crystal faces; crystal forms Exercises to be handed in: In these two labs you
More informationThis is Solids, chapter 12 from the book Principles of General Chemistry (index.html) (v. 1.0).
This is Solids, chapter 12 from the book Principles of General Chemistry (index.html) (v. 1.0). This book is licensed under a Creative Commons byncsa 3.0 (http://creativecommons.org/licenses/byncsa/
More informationAnswer: = π cm. Solution:
Round #1, Problem A: (4 points/10 minutes) The perimeter of a semicircular region in centimeters is numerically equal to its area in square centimeters. What is the radius of the semicircle in centimeters?
More information16. Let S denote the set of positive integers 18. Thus S = {1, 2,..., 18}. How many subsets of S have sum greater than 85? (You may use symbols such
æ. Simplify 2 + 3 + 4. 2. A quart of liquid contains 0% alcohol, and another 3quart bottle full of liquid contains 30% alcohol. They are mixed together. What is the percentage of alcohol in the mixture?
More informationLecture 3: Electron statistics in a solid
Lecture 3: Electron statistics in a solid Contents Density of states. DOS in a 3D uniform solid.................... 3.2 DOS for a 2D solid........................ 4.3 DOS for a D solid........................
More informationPrecession photograph
Precession photograph Spacing of spots is used to get unit cell dimensions. Note symmetrical pattern. Crystal symmetry leads to diffraction pattern symmetry. Groups Total For proteins Laue group 230 space
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS. C Zn A Cu C Zn A Cu C Cu A Zn. (30)(63.55 g /mol) (30)(63.55 g /mol) (70)(65.
HAPTER 4 IMPERFETIONS IN SOLIDS PROBLEM SOLUTIONS wt% u? 4.7 What is the composition, in atom percent, of an alloy that consists of 30 wt% Zn and 70 4.6 as In order to compute composition, in atom percent,
More informationGeometry A Solutions. Written by Ante Qu
Geometry A Solutions Written by Ante Qu 1. [3] Three circles, with radii of 1, 1, and, are externally tangent to each other. The minimum possible area of a quadrilateral that contains and is tangent to
More information1 Principles of Xray Diffraction
001_Kapitel_1 3.09.005 14:56 Uhr Seite 1 1 Principles of Xray Diffraction Diffraction effects are observed when electromagnetic radiation impinges on periodic structures with geometrical variations on
More informationGeneral tests Algebra
General tests Algebra Question () : Choose the correct answer :  If = then = a)0 b) 6 c)5 d)4  The shape which represents Y is a function of is :   V A B C D o   y   V o    V o    V o  if
More informationXRay Diffraction. wavelength Electric field of light
Light is composed of electromagnetic radiation with an electric component that modulates versus time perpendicular to the direction it is travelling (the magnetic component is also perpendicular to the
More information4. An isosceles triangle has two sides of length 10 and one of length 12. What is its area?
1 1 2 + 1 3 + 1 5 = 2 The sum of three numbers is 17 The first is 2 times the second The third is 5 more than the second What is the value of the largest of the three numbers? 3 A chemist has 100 cc of
More informationChapter 13 The Chemistry of Solids
Chapter 13 The Chemistry of Solids Jeffrey Mack California State University, Sacramento Metallic & Ionic Solids Crystal Lattices Regular 3D arrangements of equivalent LATTICE POINTS in space. Lattice
More informationIntroduction to Xray Diffraction (XRD) Learning Activity
Introduction to Xray Diffraction (XRD) Learning Activity Basic Theory: Diffraction and Bragg s Law Take a look at the diagram below: Xrays Interacting with Material A Scatter Single Particle B Diffraction
More informationUK Junior Mathematical Olympiad 2016
UK Junior Mathematical Olympiad 206 Organised by The United Kingdom Mathematics Trust Tuesday 4th June 206 RULES AND GUIDELINES : READ THESE INSTRUCTIONS CAREFULLY BEFORE STARTING. Time allowed: 2 hours.
More informationCHAPTER 29 VOLUMES AND SURFACE AREAS OF COMMON SOLIDS
CHAPTER 9 VOLUMES AND SURFACE AREAS OF COMMON EXERCISE 14 Page 9 SOLIDS 1. Change a volume of 1 00 000 cm to cubic metres. 1m = 10 cm or 1cm = 10 6m 6 Hence, 1 00 000 cm = 1 00 000 10 6m = 1. m. Change
More informationBC Exam Solutions Texas A&M High School Math Contest November 8, 2014
Exam Solutions Texas &M High School Math ontest November 8, 014 If units are involved, include them in your answer, which needs to be simplified. 1. If an arc of 60 on circle I has the same length as an
More informationCHAPTER 8, GEOMETRY. 4. A circular cylinder has a circumference of 33 in. Use 22 as the approximate value of π and find the radius of this cylinder.
TEST A CHAPTER 8, GEOMETRY 1. A rectangular plot of ground is to be enclosed with 180 yd of fencing. If the plot is twice as long as it is wide, what are its dimensions? 2. A 4 cm by 6 cm rectangle has
More informationMidterm Exam I, Calculus III, Sample A
Midterm Exam I, Calculus III, Sample A 1. (1 points) Show that the 4 points P 1 = (,, ), P = (, 3, ), P 3 = (1, 1, 1), P 4 = (1, 4, 1) are coplanar (they lie on the same plane), and find the equation of
More informationHydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules
141 CHAPTER 14 POLYMER STRUCTURES PROBLEM SOLUTIONS Hydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules 14.1 The repeat unit structures called for are sketched below. (a Polychlorotrifluoroethylene
More informationGeometry B Solutions. Written by Ante Qu
Geometry B Solutions Written by Ante Qu 1. [3] During chemistry labs, we oftentimes fold a diskshaped filter paper twice, and then open up a flap of the quartercircle to form a cone shape, as in the diagram.
More informationChapter 17. Mensuration of Pyramid
44 Chapter 7 7. Pyramid: A pyramid is a solid whose base is a plane polygon and sides are triangles that meet in a common vertex. The triangular sides are called lateral faces. The common vertex is also
More informationMAE 20 Winter 2011 Assignment 3 solutions
MAE 20 Winter 2011 Assignment 3 solutions 4.3 Calculate the activation energy for vacancy formation in aluminum, given that the equilibrium number of vacancies at 500 C (773 K) is 7.57 10 23 m 3. The
More informationUnits and Vectors: Tools for Physics
Chapter 1 Units and Vectors: Tools for Physics 1.1 The Important Stuff 1.1.1 The SI System Physics is based on measurement. Measurements are made by comparisons to well defined standards which define the
More information1. Determine all real numbers a, b, c, d that satisfy the following system of equations.
altic Way 1999 Reykjavík, November 6, 1999 Problems 1. etermine all real numbers a, b, c, d that satisfy the following system of equations. abc + ab + bc + ca + a + b + c = 1 bcd + bc + cd + db + b + c
More informationWinter 2016 Math 213 Final Exam. Points Possible. Subtotal 100. Total 100
Winter 2016 Math 213 Final Exam Name Instructions: Show ALL work. Simplify wherever possible. Clearly indicate your final answer. Problem Number Points Possible Score 1 25 2 25 3 25 4 25 Subtotal 100 Extra
More informationApplications of Trigonometry
chapter 6 Tides on a Florida beach follow a periodic pattern modeled by trigonometric functions. Applications of Trigonometry This chapter focuses on applications of the trigonometry that was introduced
More informationBryn Mawr College Department of Physics Undergraduate Teaching Laboratories Xray Crystallography
Bryn Mawr College Department of Physics Undergraduate Teaching Laboratories Xray Crystallography Introduction In this lab you will explore the Xray spectrum produced by copper in an Xray tube and investigate
More informationChapter 2: Crystal Structures and Symmetry
Chapter 2: Crystal Structures and Symmetry Laue, ravais December 28, 2001 Contents 1 Lattice Types and Symmetry 3 1.1 TwoDimensional Lattices................. 3 1.2 ThreeDimensional Lattices................
More informationSTRAIGHT LINE COORDINATE GEOMETRY
STRAIGHT LINE COORDINATE GEOMETRY (EXAM QUESTIONS) Question 1 (**) The points P and Q have coordinates ( 7,3 ) and ( 5,0), respectively. a) Determine an equation for the straight line PQ, giving the answer
More informationThe Structure of solids.
Chapter S. The Structure of solids. After having studied this chapter, the student will be able to: 1. Distinguish between a crystal structure and an amorphous structure. 2. Describe the concept of a unit
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationUsing determinants, it is possible to express the solution to a system of equations whose coefficient matrix is invertible:
Cramer s Rule and the Adjugate Using determinants, it is possible to express the solution to a system of equations whose coefficient matrix is invertible: Theorem [Cramer s Rule] If A is an invertible
More informationSolutions to Exercises, Section 6.1
Instructor s Solutions Manual, Section 6.1 Exercise 1 Solutions to Exercises, Section 6.1 1. Find the area of a triangle that has sides of length 3 and 4, with an angle of 37 between those sides. 3 4 sin
More informationPart 1. XRAY DIFFRACTION MICROSTRUCTURE ANALYSIS
5 Part 1. XRAY DIFFRACTION MICROSTRUCTURE ANALYSIS 1.1. INTERACTION OF ELECTROMAGNETIC WAVES WITH MATTER The different parts of the electromagnetic spectrum have very different effects upon interaction
More informationHCP crystal planes are described using the MillerBravais indices, (hkil) Draw the hexagonal crystal planes whose MillerBravais indices are:
.6 How re crystllogrphic plnes indicted in HCP unit cells? In HCP unit cells, crystllogrphic plnes re indicted using four indices which correspond to four xes: three bsl xes of the unit cell,,, nd, which
More informationIntroduction to symmetry
130320  Some handout slides are hidden @13, @43, 3 more at the end. Introduction to symmetry 1 Recap 1/ to understand function, we need structure; to get structure, we need xray crystallography 2/ remarkable
More informationHigher Geometry Problems
Higher Geometry Problems ( Look up Eucidean Geometry on Wikipedia, and write down the English translation given of each of the first four postulates of Euclid. Rewrite each postulate as a clear statement
More informationMath 115 Spring 2014 Written Homework 10SOLUTIONS Due Friday, April 25
Math 115 Spring 014 Written Homework 10SOLUTIONS Due Friday, April 5 1. Use the following graph of y = g(x to answer the questions below (this is NOT the graph of a rational function: (a State the domain
More informationHomework from Section Find two positive numbers whose product is 100 and whose sum is a minimum.
Homework from Section 4.5 4.5.3. Find two positive numbers whose product is 100 and whose sum is a minimum. We want x and y so that xy = 100 and S = x + y is minimized. Since xy = 100, x = 0. Thus we have
More informationSTRAIGHT LINES. , y 1. tan. and m 2. 1 mm. If we take the acute angle between two lines, then tan θ = = 1. x h x x. x 1. ) (x 2
STRAIGHT LINES Chapter 10 10.1 Overview 10.1.1 Slope of a line If θ is the angle made by a line with positive direction of xaxis in anticlockwise direction, then the value of tan θ is called the slope
More information